Active Standard ASTM A913 / A913M | Developed by Subcommittee: A01.02
Book of Standards Volume: 01.04
Historical (view previous versions of standard)
This specification covers high-strength low-alloy steel shapes of structural quality, produced by quenching and self-tempering process (QST). The chemical analysis of the heat and of the steel product analysis shall conform to the chemical requirements prescribed by the reference materials. The Charpy V-notch test shall be performed to determine if the material conforms to the required tensile properties.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers high-strength low-alloy structural steel shapes in Grades 50 , 60 , 65  and 70 , produced by the quenching and self-tempering process (QST). The shapes are intended for riveted, bolted or welded construction of bridges, buildings and other structures.
1.2 The QST process consists of in line heat treatment and cooling rate controls which result in mechanical properties in the finished condition that are equivalent to those attained using heat treating processes which entail reheating after rolling. A description of the QST process is given in Appendix X1.
1.3 Due to the inherent characteristics of the QST process, the shapes shall not be formed and post weld heat treated at temperatures exceeding 1100°F [600°C].
1.4 When the steel is to be welded, it is presupposed that a welding procedure suitable for the grade of steel and intended use or service will be utilized. See Appendix X3 of Specification A6/A6M for information on weldability.
1.5 The values stated in either inch-pound units or SI units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with this specification.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A6/A6M Specification for General Requirements for Rolled Structural Steel Bars, Plates, Shapes, and Sheet Piling
A673/A673M Specification for Sampling Procedure for Impact Testing of Structural Steel
A898/A898M Specification for Straight Beam Ultrasonic Examination of Rolled Steel Structural Shapes
ICS Number Code 77.140.70 (Steel profiles)